| ||Format||Pages||Price|| |
|3||$39.00||  ADD TO CART|
|Hardcopy (shipping and handling)||3||$39.00||  ADD TO CART|
|Standard + Redline PDF Bundle||6||$46.80||  ADD TO CART|
Significance and Use
The void content of a composite may significantly affect some of its mechanical properties. Higher void contents usually mean lower fatigue resistance, greater susceptibility to water penetration and weathering, and increased variation or scatter in strength properties. The knowledge of void content is desirable for estimation of quality of composites.
1.1 These test methods cover the void content of reinforced plastics or “composites.” The test methods are applicable to composites for which the effects of ignition on the materials are known. Most plastics, glass, and reinforcements fall into this class. These test methods are not applicable to composites for which the effects of ignition on the plastics, the reinforcement, and any fillers are unknown. This class may include silicone resins, which do not burn off completely, reinforcements consisting of metals, organic materials, or inorganic materials which may gain or lose weight, and fillers consisting of oxides, carbonates, etc., which may gain or lose weight. Note that separate weight loss tests of individual materials will usually, but not necessarily, give the same result as when all the materials are combined.
Note 1—There is no known ISO equivalent to these test methods.
1.2 The values stated in SI units are to be regarded as standard.
1.3 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
D618 Practice for Conditioning Plastics for Testing
D792 Test Methods for Density and Specific Gravity (Relative Density) of Plastics by Displacement
D1505 Test Method for Density of Plastics by the Density-Gradient Technique
D2584 Test Method for Ignition Loss of Cured Reinforced Resins
ICS Number Code 83.120 (Reinforced plastics)
UNSPSC Code 13100000(Rubber and elastomers)
ASTM D2734-09, Standard Test Methods for Void Content of Reinforced Plastics, ASTM International, West Conshohocken, PA, 2009, www.astm.orgBack to Top